Improving accuracy of interatomic potentials: more physics or more data? A case study of silica. Ivan S. Novikova , Alexander V. Shapeeva,∗ a

Skolkovo Institute of Science and Technology, Skolkovo Innovation Center, Nobel St. 3, Moscow 143026, Russia

Abstract In this paper we investigate the extent to which a charge-equilibration (QEq) model can improve the accuracy of interatomic potentials in general, and a machine-learning potential in particular. To that end, we compare three kinds of interatomic potentials: the Stillinger-Weber (SW) potential, the SW potential combined with the QEq model (SW+QEq) and the Moment Tensor Potential (MTP) fitted to a DFT dataset of α-quartz SiO2 -based structures. In order to make a meaningful comparison, in addition to the accuracy, we assess the uncertainty of predictions of each potential. It is shown that MTP has the lowest error and uncertainty among the three potentials. Moreover, adding the QEq model to MTP does not make any improvement over the MTP potential alone. Keywords: charge-equilibration model; Stillinger-Weber potential; machine-learning interatomic potentials; Moment Tensor Potential; uncertainty quantification 1. Introduction Oxides represent one of the most important class of functional materials deriving their unique properties from the nature of ionic bonding of oxygen. Silicon dioxide (SiO2 , silica), although not rated as a functional material, has been extensively studied as it has many industrial applications including semiconductors [1], metal casting [2], and in the production of glass [3], ∗

Corresponding author Email address: [email protected] (Alexander V. Shapeev)

Preprint submitted to Computational Materials Science

August 11, 2018

to name a few. In addition to experimental works [4, 5, 6], there has been extensive efforts in studying SiO2 computationally. Density functional theory (DFT) is able to correctly describe ionic bonds and Coulombic interaction and hence provides an accurate description of interatomic interaction in the SiO2 system. However, DFT is too computationally expensive to model some of the critical properties of SiO2 such as the solidification of molten silicon, for which the interaction model has to be several orders of magnitude more computationally efficient. (Semi-)empirical interatomic potentials has thus been the only alternative to DFT for conducting large-scale simulations of SiO2 . Examples of such potentials are the Stillinger-Weber (SW) potential [7, 8] and the Tersoff potential [9]. These potentials have a relatively simple functional form for the short-range interatomic interactions and they do not explicitly capture long-range Coulombic interactions in oxides. For example, the SW potential is a pair-interaction potential with a three-body term penalizing the bond angles that differ from the ones expected to occur in SiO2 . Many efforts have been made to put more physics into the model to make it more accurate. For instance, fixed-charge pair potentials combining short-range and long-range interactions have been proposed in [10, 11]. However, such the potentials cannot readjust to match the electrostatic environment. In [12, 13] the above fixed-charge potentials were extended. In those interatomic interaction models the charges became the parameters which were optimized and the effects of dipole polarization of the oxygen ions were taken into account. The charge equilibration (QEq) model is a more sophisticated model proposed by Rappe and Goddard [14]. QEq allows the charges to respond to changes in the electrostatic environment. Some interatomic interaction models, such as modified Tersoff [15], ReaxFF [16] and COMB [17] were constructed on the basis of the QEq model. These potentials have been successfully used in the description of SiO2 . However, application of these potentials to large-scale systems may be limited due to the fact that the QEq method requires a significantly larger computational effort than conventional empirical potentials. Another research direction intended to increase the accuracy of the interatomic potentials is the so-called machine-learning interatomic potentials [18, 19, 20, 21, 22, 23, 24, 25, 26, 27, 28, 29, 30, 31, 32, 33, 34, 35, 36, 37, 38, 39, 40, 41]. Ideologically, they are different from the empirical interatomic potentials in the way that machine-learning potentials attempt to increase accuracy not by putting more physics into the model, but through a flexible 2

functional form that allows large amounts of DFT data to be used for the fitting. The first work on this topic was published by Behler and Parinello [18]. They constructed a neural network potential (NNP) and successfully applied it to modelling of silicon; in particular, their potential predicted the radial distribution function of a silicon melt at 3000 K with high accuracy. In [19] on the basis of the idea of Gaussian process regression, the Gaussian approximation potential (GAP) was proposed and successfully applied for prediction of various properties of carbon, silicon and germanium. Thereafter, many works appeared that propose or validate interatomic potentials based on neural networks [25, 26, 27, 21, 28, 29, 30, 31, 32, 33, 34, 42], Gaussian processes [20, 35, 36, 37] and other methods [22, 23, 24, 38]. In the above works only short-range interaction was taken into account. Behler and his collaborators extended their NNP by including electrostatic interactions explicitly in the functional form [43] and testing it for ZnO, not reporting, however, that it improves the accuracy of their potential. A similar model directly predicting atomic charges has recently been proposed in [44]. The field of machine-learning interatomic potentials is ideologically and methodologically close to the field of machine-learning cheminformatics—developing of models predicting the properties of molecules and materials directly, without a molecular simulation [45, 46, 47, 48, 49, 50, 51, 52, 53]. Many studies on machine-learning potentials report [18, 19, 20, 28, 33, 35] that these potentials are more accurate than off-the-shelf empirical potentials. A conceptually interesting study was [20], where the authors considered a growing set of quantities of interest (phonons, elastic constants, defects, surfaces, etc.) and show that it is possible to construct a series of potentials that reproduce this growing set without losing accuracy by increasing the number of parameters in a potential. The most closely related paper to this study is [21]. In this paper the authors show that when the potentials are fitted on a very large configurational space (containing bulk, surfaces, clusters, etc.) for pure gold, a machine-learning potential was significantly more accurate than ReaxFF. However, gold has largely delocalized metallic bonds that are hard to represent explicitly in an empirical potential with high accuracy. On the other hand, SiO2 has ionic/covalent bonding which empirical potentials are expected to represent sufficiently accurately. The main purpose of this work was to assess to what extent the accuracy can be increased by adding a charge equilibration model (and hence capture the ionic nature of SiO2 bonding better) to an interatomic potential in general, and a machine-learning potential in particular. In order to answer that 3

question, we compare three different potentials, the Stillinger-Weber (SW) potential, the SW potential with the additional charge equilibration model (SW+QEq) and the Moment Tensor Potential (MTP), belonging to a class of machine-learning potentials. MTP was first proposed in [22] for the case of single-component materials and extended in [23, 24] to multi-component materials. This paper is organized as follows. In Section 2 we describe the methodology namely, the interatomic potentials, their fitting, and our uncertainty quantification method. In Section 3 we present and discuss the results of numerical experiments. In particular, we compare the training errors in energies, forces and stresses for different models, as well as elastic constants, vacancy formation energies (VFEs), phonon spectra and radial distribution functions (RDFs) obtained by these models. Finally, in Section 4 we give the concluding remarks. 2. Methodology In order to address the main question of this study, namely to what extent the accuracy of the description of ionic bonds can be improved by adding a charge-equilibration (QEq) model, we introduce the SW potential, the QEq model, and the MTP potential (Section 2.1). Since our main focus is the machine-learning potentials, we consider a local optimization method for finding the parameters (Section 2.2). Finally, to in order to better analyze the results, we introduce an uncertainty quantification method in Section 2.3. 2.1. Interatomic potentials We start by formulating an SW potential in the form similar to the one from [8]. The potential has originally been developed to describe bulk silicon [54]. It expresses local interaction of atoms and does not explicitly account for the Coulombic long-range interactions. Let x = {(xi , zi ) : i = 1, . . . , n} be a configuration with n atoms, each atom is encoded by its position xi and atomic type zi . We assume that the i-th atom interacts with its neighbors and we refer to the j-th atom as the neighbor of the i-th atom if the distance between them is not greater than a cutoff radius Rcut . The locality of interaction is expressed by expanding the total interaction energy as a sum of contributions of individual atoms P P (or, to be precise, individual atomic neighborhoods): E(x) = i Vi := i V (ri ), where ri = (ri 1 , . . . , rij , . . . , ri n ) is

4

the neighborhood of the i-th atom, rij = xj − xi is the position of the j-th atom relative to the i-th atom. We generalize the SW potential by allowing its radial and angular functions to be arbitrary. To that end, we introduce a radial basis ( T α (r)(Rcut − r)2 r < Rcut ϕα (r) = (1) 0 r ≥ Rcut , where T α (r) is the Chebyshev polynomial of degree α on the interval [Rmin , Rcut ], the term (Rcut − r)2 is introduced to ensure a smooth cutoff to 0 at r ≥ Rcut , and Rmin is some lower bound on minimal interatomic distances. For illustration, we plot the first six radial basis functions on the interval [1.5 ˚ A, 5 ˚ A] in Figure 1. 15

φ1 φ2 φ3 φ4 φ5 φ6

10

φ(r)

5 0 −5 −10 −15

1.5

2

2.5

3

3.5

4

4.5

5

r, Å

Figure 1: Radial basis ϕ1 , . . . , ϕ6 .

Next we define the contribution ViSW of each atom: ViSW := ViSW2 + ViSW3 , (2) X X 1 cβ,zi zj ϕβ (|rij |), ViSW2 = 2 j β X X 1 XX ViSW3 = λzi zj zk (cos θijk + θ˜zi zj zk )2 c˜β,zi zj ϕβ (|rij |) c˜γ,zi zk ϕγ (|rik |), 2 j k

Skolkovo Institute of Science and Technology, Skolkovo Innovation Center, Nobel St. 3, Moscow 143026, Russia

Abstract In this paper we investigate the extent to which a charge-equilibration (QEq) model can improve the accuracy of interatomic potentials in general, and a machine-learning potential in particular. To that end, we compare three kinds of interatomic potentials: the Stillinger-Weber (SW) potential, the SW potential combined with the QEq model (SW+QEq) and the Moment Tensor Potential (MTP) fitted to a DFT dataset of α-quartz SiO2 -based structures. In order to make a meaningful comparison, in addition to the accuracy, we assess the uncertainty of predictions of each potential. It is shown that MTP has the lowest error and uncertainty among the three potentials. Moreover, adding the QEq model to MTP does not make any improvement over the MTP potential alone. Keywords: charge-equilibration model; Stillinger-Weber potential; machine-learning interatomic potentials; Moment Tensor Potential; uncertainty quantification 1. Introduction Oxides represent one of the most important class of functional materials deriving their unique properties from the nature of ionic bonding of oxygen. Silicon dioxide (SiO2 , silica), although not rated as a functional material, has been extensively studied as it has many industrial applications including semiconductors [1], metal casting [2], and in the production of glass [3], ∗

Corresponding author Email address: [email protected] (Alexander V. Shapeev)

Preprint submitted to Computational Materials Science

August 11, 2018

to name a few. In addition to experimental works [4, 5, 6], there has been extensive efforts in studying SiO2 computationally. Density functional theory (DFT) is able to correctly describe ionic bonds and Coulombic interaction and hence provides an accurate description of interatomic interaction in the SiO2 system. However, DFT is too computationally expensive to model some of the critical properties of SiO2 such as the solidification of molten silicon, for which the interaction model has to be several orders of magnitude more computationally efficient. (Semi-)empirical interatomic potentials has thus been the only alternative to DFT for conducting large-scale simulations of SiO2 . Examples of such potentials are the Stillinger-Weber (SW) potential [7, 8] and the Tersoff potential [9]. These potentials have a relatively simple functional form for the short-range interatomic interactions and they do not explicitly capture long-range Coulombic interactions in oxides. For example, the SW potential is a pair-interaction potential with a three-body term penalizing the bond angles that differ from the ones expected to occur in SiO2 . Many efforts have been made to put more physics into the model to make it more accurate. For instance, fixed-charge pair potentials combining short-range and long-range interactions have been proposed in [10, 11]. However, such the potentials cannot readjust to match the electrostatic environment. In [12, 13] the above fixed-charge potentials were extended. In those interatomic interaction models the charges became the parameters which were optimized and the effects of dipole polarization of the oxygen ions were taken into account. The charge equilibration (QEq) model is a more sophisticated model proposed by Rappe and Goddard [14]. QEq allows the charges to respond to changes in the electrostatic environment. Some interatomic interaction models, such as modified Tersoff [15], ReaxFF [16] and COMB [17] were constructed on the basis of the QEq model. These potentials have been successfully used in the description of SiO2 . However, application of these potentials to large-scale systems may be limited due to the fact that the QEq method requires a significantly larger computational effort than conventional empirical potentials. Another research direction intended to increase the accuracy of the interatomic potentials is the so-called machine-learning interatomic potentials [18, 19, 20, 21, 22, 23, 24, 25, 26, 27, 28, 29, 30, 31, 32, 33, 34, 35, 36, 37, 38, 39, 40, 41]. Ideologically, they are different from the empirical interatomic potentials in the way that machine-learning potentials attempt to increase accuracy not by putting more physics into the model, but through a flexible 2

functional form that allows large amounts of DFT data to be used for the fitting. The first work on this topic was published by Behler and Parinello [18]. They constructed a neural network potential (NNP) and successfully applied it to modelling of silicon; in particular, their potential predicted the radial distribution function of a silicon melt at 3000 K with high accuracy. In [19] on the basis of the idea of Gaussian process regression, the Gaussian approximation potential (GAP) was proposed and successfully applied for prediction of various properties of carbon, silicon and germanium. Thereafter, many works appeared that propose or validate interatomic potentials based on neural networks [25, 26, 27, 21, 28, 29, 30, 31, 32, 33, 34, 42], Gaussian processes [20, 35, 36, 37] and other methods [22, 23, 24, 38]. In the above works only short-range interaction was taken into account. Behler and his collaborators extended their NNP by including electrostatic interactions explicitly in the functional form [43] and testing it for ZnO, not reporting, however, that it improves the accuracy of their potential. A similar model directly predicting atomic charges has recently been proposed in [44]. The field of machine-learning interatomic potentials is ideologically and methodologically close to the field of machine-learning cheminformatics—developing of models predicting the properties of molecules and materials directly, without a molecular simulation [45, 46, 47, 48, 49, 50, 51, 52, 53]. Many studies on machine-learning potentials report [18, 19, 20, 28, 33, 35] that these potentials are more accurate than off-the-shelf empirical potentials. A conceptually interesting study was [20], where the authors considered a growing set of quantities of interest (phonons, elastic constants, defects, surfaces, etc.) and show that it is possible to construct a series of potentials that reproduce this growing set without losing accuracy by increasing the number of parameters in a potential. The most closely related paper to this study is [21]. In this paper the authors show that when the potentials are fitted on a very large configurational space (containing bulk, surfaces, clusters, etc.) for pure gold, a machine-learning potential was significantly more accurate than ReaxFF. However, gold has largely delocalized metallic bonds that are hard to represent explicitly in an empirical potential with high accuracy. On the other hand, SiO2 has ionic/covalent bonding which empirical potentials are expected to represent sufficiently accurately. The main purpose of this work was to assess to what extent the accuracy can be increased by adding a charge equilibration model (and hence capture the ionic nature of SiO2 bonding better) to an interatomic potential in general, and a machine-learning potential in particular. In order to answer that 3

question, we compare three different potentials, the Stillinger-Weber (SW) potential, the SW potential with the additional charge equilibration model (SW+QEq) and the Moment Tensor Potential (MTP), belonging to a class of machine-learning potentials. MTP was first proposed in [22] for the case of single-component materials and extended in [23, 24] to multi-component materials. This paper is organized as follows. In Section 2 we describe the methodology namely, the interatomic potentials, their fitting, and our uncertainty quantification method. In Section 3 we present and discuss the results of numerical experiments. In particular, we compare the training errors in energies, forces and stresses for different models, as well as elastic constants, vacancy formation energies (VFEs), phonon spectra and radial distribution functions (RDFs) obtained by these models. Finally, in Section 4 we give the concluding remarks. 2. Methodology In order to address the main question of this study, namely to what extent the accuracy of the description of ionic bonds can be improved by adding a charge-equilibration (QEq) model, we introduce the SW potential, the QEq model, and the MTP potential (Section 2.1). Since our main focus is the machine-learning potentials, we consider a local optimization method for finding the parameters (Section 2.2). Finally, to in order to better analyze the results, we introduce an uncertainty quantification method in Section 2.3. 2.1. Interatomic potentials We start by formulating an SW potential in the form similar to the one from [8]. The potential has originally been developed to describe bulk silicon [54]. It expresses local interaction of atoms and does not explicitly account for the Coulombic long-range interactions. Let x = {(xi , zi ) : i = 1, . . . , n} be a configuration with n atoms, each atom is encoded by its position xi and atomic type zi . We assume that the i-th atom interacts with its neighbors and we refer to the j-th atom as the neighbor of the i-th atom if the distance between them is not greater than a cutoff radius Rcut . The locality of interaction is expressed by expanding the total interaction energy as a sum of contributions of individual atoms P P (or, to be precise, individual atomic neighborhoods): E(x) = i Vi := i V (ri ), where ri = (ri 1 , . . . , rij , . . . , ri n ) is

4

the neighborhood of the i-th atom, rij = xj − xi is the position of the j-th atom relative to the i-th atom. We generalize the SW potential by allowing its radial and angular functions to be arbitrary. To that end, we introduce a radial basis ( T α (r)(Rcut − r)2 r < Rcut ϕα (r) = (1) 0 r ≥ Rcut , where T α (r) is the Chebyshev polynomial of degree α on the interval [Rmin , Rcut ], the term (Rcut − r)2 is introduced to ensure a smooth cutoff to 0 at r ≥ Rcut , and Rmin is some lower bound on minimal interatomic distances. For illustration, we plot the first six radial basis functions on the interval [1.5 ˚ A, 5 ˚ A] in Figure 1. 15

φ1 φ2 φ3 φ4 φ5 φ6

10

φ(r)

5 0 −5 −10 −15

1.5

2

2.5

3

3.5

4

4.5

5

r, Å

Figure 1: Radial basis ϕ1 , . . . , ϕ6 .

Next we define the contribution ViSW of each atom: ViSW := ViSW2 + ViSW3 , (2) X X 1 cβ,zi zj ϕβ (|rij |), ViSW2 = 2 j β X X 1 XX ViSW3 = λzi zj zk (cos θijk + θ˜zi zj zk )2 c˜β,zi zj ϕβ (|rij |) c˜γ,zi zk ϕγ (|rik |), 2 j k